Enhancement of the water-resistance properties of an edible film prepared from mung bean starch via the incorporation of sunflower seed oil

Mung bean starch (MBS)-based edible films with incorporation of guar gum (GG) and sunflower seed oil (SSO) were developed in this study. MBS, GG, and SSO were used as the main filmogenic biopolymer, thickener, and hydrophobicity-imparting substance, respectively. To investigate the effect of SSO content on the physicochemical, mechanical, and optical properties of the films, they were supplemented with various concentrations (0, 0.5, 1, and 2%, w/w) of SSO. Increasing SSO content tended to decrease tensile strength, elongation at break, crystallinity, water solubility, and the water vapor permeability; in contrast, it increased the oxygen transmission rate and water contact angle. Consequently, the incorporation of SSO into the matrix of MBS-based films decreased their mechanical strength but effectively enhanced their water-resistance properties. Therefore, the MBS-based film developed here can be properly used as an edible film in settings that require high water-resistance properties but do not call for robust mechanical strength.


Formation of SSO/GG/MBS composite films. SSO/GG/MBS composite films were prepared as shown in
. An MBS suspension (4%, w/w) was prepared with distilled water and heated at 90-95 ℃ by stirring for 30 min. The MBS suspension was then cooled to room temperature (RT; 22 ± 3 °C) with mild stirring. A GG dispersion (1.5%, w/w) in distilled water was manufactured using a high-speed homogenizer (SR30; M-TOPS Co., Ltd., Yangju, Korea) at 15,000 rpm at RT until agglomeration of the GG was completely broken. Subsequently, the prepared MBS suspension and GG dispersion were blended and stirred at RT for 45 min. Glycerol [30% (w/w) of the solid content of the mixture of MBS suspension and GG dispersion (GG/MBS mixture)] was then added to GG/MBS mixture and stirred at RT for 15 min. SSO was added to the resulting mixture at various concentrations [0, 0.5, 1, and 2% (w/w) of the weight of GG/MBS mixture] and homogenized using a high-speed homogenizer (SR30; M-TOPS Co., Ltd.) at 15,000 rpm at RT for 3 min. To remove air bubbles, the filmogenic emulsions were degassed in a vacuum chamber (VS-1202V5; Vision Scientific Co., Ltd., Bucheon, Korea) at RT for 30 min. The films were elaborated using the casting technique. The degassed filmogenic emulsions (9.82 mg of solids cm −2 ) were gently poured over square Petri dishes (polystyrene, 12.5 × 12.5 cm) resting on a leveled surface and dried at 40 °C and 25% relative humidity (RH) for 24 h. The same dry matter density of filmogenic emulsions was dispensed to obtain a constant film thickness. The dried films were carefully peeled off the casting dishes and conditioned at 25 °C and 50% RH for at least 48 h in a thermo-hygrostat (Labmade 011; Sejong Scientific Co., Ltd., Bucheon, Korea) before the analysis of their properties.
Characterization of the composite films. Thickness and mechanical properties. The thickness (μm) of the films was measured using a digimatic indicator (ID-C112X; Mitutoyo Corp., Kanagawa, Japan) with a precision of 0.001 mm at 10 random positions on the film.
The specimens used for measuring the mechanical properties of the films were cut into 25.4 × 100 mm rectangles. The tensile strength (TS) and elongation at break (EB) parameters of each film were investigated using a universal testing machine (Instron 3366; Instron Engineering Corp., Norwood, MA, USA) operated with a load cell of 5 kN, an initial grip separation of 50 mm, and a cross-head speed of 500 mm min −1 , according to the ASTM D882-02 standard test method. For each film sample, five specimens were measured.
Optical properties. Color. The color of the films was assessed using a colorimeter (CR-400; Konica Minolta Sensing, Inc., Osaka, Japan) that was calibrated using a standard white plate (Y = 93.8, x = 0.3131, and y = 0.3191). The films were placed on the standard white plate, and the CIE L * a * b * values were recorded at five random locations on the film surface. The total color difference ( E * ), hue angle (H°), and chroma (C * ) were calculated using the following equations (Eqs. [1][2][3].
Structural properties. Fourier transform infrared (FT-IR) spectroscopy. The FT-IR spectra of pure SSO and GG/MBS and SSO/GG/MBS composite films were obtained using an FT-IR spectrometer (Cary 630; Agilent Technologies, Inc., Santa Clara, CA, USA) in the attenuated total reflectance mode. All spectra were recorded in the range of 4,000-600 cm −1 at a resolution rate of 4 cm −1 by co-adding 128 scans.
X-ray diffraction (XRD). The XRD patterns of GG and MBS granules and GG/MBS and SSO/GG/MBS composite films were obtained using an X-ray diffractometer (X'Pert PW3040/00; Malvern Panalytical Ltd., Worcestershire, Malvern, UK) equipped with Cu Kα radiation (λ = 1.5406 Å). The XRD patterns were recorded at a step size of 0.0170°, a scan step time of 45.72 s, and a scan rate of 2° min −1 , operated at a voltage of 40 kV and a current of 30 mA.
Morphological properties. The film surface and cross-section morphologies were characterized using a scanning electron microscope (SEM) (SU-70; Hitachi Ltd., Tokyo, Japan). The films samples were cut by a razor blade and coated with platinum for 70 s and observed with an accelerating voltage of 20 kV.
Oxygen transmission rate (OTR). The OTR of the films was examined using an oxygen permeation analyzer (8003; Systech Instruments Ltd., Illinois, Johnsburg, IL, USA), according to the ASTM D3895-05 standard test method at 23 °C and 0% RH. The specimens were mounted onto the diffusion cells and exposed to pure oxygen flow on one side, with pure nitrogen flow on the other side. The area of exposure during the test was 56.745 cm 2 for each sample. Measurements were performed in duplicate and are expressed as the quantity of oxygen molecules passing through the 1 m 2 of the film surface area over 1 day.
Water-resistance properties. Preparation of commercial starch-based edible film. To compare water-resistance properties of SSO/GG/MBS composite films with commercial edible film, starch-based edible film on the market (Oblate; Daewha Food, Gimpo, Korea) was also prepared. The oblate film was made of potato starch, corn starch, and soybean phospholipid, and its thickness was 36.10 ± 1.37 µm.
Moisture content. Films were cut into square specimens of 20 × 20 mm, and initial weight was measured. Subsequently, the films were dried in a drying oven (VS 41720; Vision Scientific Co., Ltd., Daejeon, Korea) at 105 °C for 24 h. The moisture content was calculated using Eq. (5) as follows: where W w was the initial weight of the film and W d was the constant weight of the film after drying at 105 °C for 24 h. Five replicates were performed for each film.
Water solubility. The films (20 × 20 mm) were dried in the drying oven (VS 41720; Vision Scientific Co., Ltd.), and the weight of the dried films was determined. Subsequently, the dried films were immersed in 50 mL of distilled water at 25 °C for 24 h. The wet films were re-dried in the drying oven (VS 41720; Vision Scientific Co., Ltd.) at 105 °C for 24 h to obtain their final dry mass. The water solubility of the films was calculated using Eq. (6) as follows: where W i and W f were the initial and final dry weight of the films, respectively.
Water vapor permeability (WVP). WVP of the packaging films in one of their most significant properties to determine their fitness for use as packaging materials 14 . In addition, WVP is an important property to characterize the overall water-resistance properties of the films 15 . Therefore, the WVP was considered as the representative attribute in the water-resistance properties of the SSO/GG/MBS composite films. To study the effect of storage time on the WVP in the SSO/GG/MBS composite films, films were stored at 25 °C and 50% RH for 14 days in a thermo-hygrostat (Labmade 011; Sejong Scientific Co., Ltd.). The WVP values in the films were analyzed on days 0, 2, 5, 9, and 14. WVP was determined gravimetrically according to ASTM E96-05 standard test method. Films cut into circles with a diameter of 65 mm were mounted onto poly(methyl methacrylate) cups (diameter, 45 mm) previously filled with 15 g of calcium chloride dehydrate, with the smooth and shiny side of the film facing outward. Three where W is the variation in the weight of the cup (g) after 24 h, x is the thickness of the film (mm), A is the exposed permeation area (0.00159 m 2 ) of the film, t is the elapsed time (1 day), and P is the water vapor partial pressure differences across the film.
Wettability of the film surface. To analyze the surface wettability of the films, the water contact angle on the surface of the films was measured using the sessile drop method and a drop shape analyzer (DSA25; KRÜSS GmbH, Hamburg, Germany). A droplet of distilled water (3 μL) was formed at the tip of a syringe needle and carefully deposited onto the top of the surface of the films at RT. The measurements were repeated at three different points on each film sample.
Statistical analysis. Data analyses were carried out using Statistical Package for the Social Sciences (SPSS) software version 25.0 (SPSS, Inc., Chicago, IL, USA). The significant differences (P ≤ 0.05) among result values in the SSO/GG/MBS films in the measurements of their characteristics [thickness, mechanical properties (tensile strength and elongation at break), optical properties (L * , a * , b * , ΔE * , H°, C * , and transparency), OTR, water-resistance properties (moisture content, water solubility, WVP, and wettability of the film surface)] were identified using one-way analysis (ANOVA) followed by Duncan's multiple range tests. All data are presented as mean ± standard deviation from a minimum of three replicates.

Results and discussion
thickness and mechanical properties. The resulting thickness and mechanical properties of the GG/ MBS and SSO/GG/MBS composite films are presented in Table 1. There were no significant differences (P > 0.05) in thickness among all film formulations, because the quantity of filmogenic emulsion of each formulation that was poured onto the plate was calculated to the constant weight of solid content for films with a thickness of 92 μm. TS and EB are essential characteristics of packaging materials 16 . The addition of SSO to the GG/MBS films caused a significant reduction (P ≤ 0.05) in TS and EB. Generally, the incorporation of an appropriate level of oils into a film matrix decreases TS but increases EB. This phenomenon can be explained by the plasticizer effect of the oil on the film matrix. The oil incorporated into the film matrix is responsible for the partial substitution of strong intermolecular polymer-polymer interactions with weak intermolecular polymer-oil interactions in the film matrix, resulting in heterogeneity of the film structure, featuring discontinuities 17 . The oil diminishes the cohesion of the polymer network forces and extends the amorphous regions of the film matrix. The decrease in film crystallinity decreases the mechanical strength 18 . Evidence of the increase in the amorphous phase in the SSO/GG/MBS composite films as the SSO content increased is provided in subsection "XRD". Therefore, the addition of oil to films, to a certain extent, decreases the rigidity and increases the flexibility of the film. This phenomenon is the plasticizing action of oils. However, in this study, both TS and EB were reduced in SSO/GG/ MBS composite films compared with those in GG/MBS films. This result can be explained by the surfactantfree effect in oil-in-water type filmogenic emulsion. Oil-in-water emulsions are unstable without any added surfactant, and was separated into oil and water phases if it left with no agitation 19 . Therefore, surfactants are used to stabilize the dispersion state in the oil-in-water emulsions. Surfactants can improve the stability in oilin-water emulsions by enhancing the compatibility between hydrophilic and hydrophobic phases. However, in our study, the surfactant was not used to fabricate the SSO/GG/MBS composite films. The developed films were edible films, and these were needed to retain stability when ingested by the human body. Therefore, the SSO/ GG/MBS composite films did not contain any surfactant materials. Accordingly, in the SSO/GG/MBS composite filmogenic emulsions, blend of the SSO (hydrophobic phase) and GG/MBS mixture (hydrophilic phase) was not adequately occurred because they did not contain no surfactant. Surfactant-free oil-in-water emulsions typically generate much larger oil droplets 20 . This phenomenon caused the discontinuities in the film matrix, and lead to a decrease in tensile strength and elongation at break values 21 . Relatively large amount of SSO that was added to films, which induced SSO agglomeration and caused a considerable local concentration stress 22 . For this reason, EB in SSO/GG/MBS composite films was decreased by the addition of SSO. The results of SEM analysis provided optical properties. Edible films are applied directly to food surfaces in wrapping or coating form. Therefore, the color and transparency of edible films are significant factors for the visual appearance and consumer acceptance of foods. The color values of our film, including the CIE L * a * b * , H°, and C * values, are shown in Table 2. The addition of SSO to the SSO/GG/MBS composite films caused a decrease in the a * values and an increase in the b * values, suggesting that the SSO/GG/MBS composite films have more greenish-yellow tones compared with the GG/MBS film, which was attributable to the slight amber color of SSO. However, to the naked eye, there were no noticeable differences in visual appearance among the film samples. The transparency of the films decreased significantly as the amount of SSO increased. This phenomenon resulted from the increase in diffuse reflectance caused by light scattering in the oil droplet within the film structure 11 . In addition, sweating-out (or exudation) of glycerol from the film matrix to the surface may also affect the decrease in transparency of the SSO/GG/MBS composite films. Figure 2A,B show the surface appearance of 2% SSO/GG/MBS (sample with the maximum amount of SSO added) and GG/MBS (sample without SSO) films, respectively. As shown in Fig. 2A,B, sweating-out of the glycerol from the inside to the surface of the 2% SSO/GG/MBS film was demonstrated with the naked eyes. The intermolecular MBS-GG interactions were diminished as SSO content increased in the SSO/GG/MBS composite films. Therefore, the glycerol dispersed inside the film matrix in the 2% SSO/GG/MBS film was not immobilized and migrated to the surface of the film. On the contrary, there are no sweating-out of the glycerol in the GG/MBS film, since the intermolecular MBS-GG interactions were adequately formed in the film matrix. As a result, the glycerol in the GG/MBS film was well dispersed and entrapped inside the matrix. The behavior of glycerol in the 2% SSO/GG/MBS and GG/ MBS films was presented schematically in Fig. 2C,a,b, respectively. The sweating-out phenomenon of glycerol will be mentioned in later subsections "OTR" and "Wettability of the film surface". Meanwhile, Gao et al. 24 and Phupoksakul et al. 25 also reported the decrease in transparency of the film by sweating-out of glycerol. The reduction in transparency (or increase in opacity) of SSO/GG/MBS composite films could be advantageous, as opaque films can effectively block UV radiation. UV exclusion is important for prolonging the shelf-life of lipid-rich foods, which are vulnerable to the oxidative degradation catalyzed by UV radiation 26 . Structural properties. FT-IR spectroscopy. The FT-IR spectra of SSO, GG/MBS films, and SSO/GG/MBS composite films are plotted in Fig. 3A. The spectra of SSO (Fig. 3A,a) exhibited a broad band at 3,004 cm −1 that was attributed to =CH stretching. The two peaks detected at 2,921 and 2,852 cm −1 are assigned because of the CH stretching. The peaks detected at 1,743 and 1,462 cm −1 represented the ester C=O stretching of the triglyceride and CH deformation, respectively. The peak observed at 1,236 cm −1 indicated the bending of CH 2 groups. The peak 722 cm −1 was related to a C-H out-of-plane deformation 27 . These peaks, which were derived from SSO, were detected in all SSO/GG/MBS composite films, and their intensity increased with SSO concentration. The spectra of the GG/MBS film (Fig. 3A,b) 30,31 . The bands at 1,651 cm −1 were attributed to the moisture absorbed in the amorphous regions of the films. Therefore, the intensity of this peak indicates the moisture content, which exhibited a decreasing trend with the increasing content of SSO 7 . This interpretation was consistent with www.nature.com/scientificreports/ the results of the moisture content analysis of the films (subsection "Moisture content"). Compared with the spectra of the GG/MBS film (Fig. 3A,b) and of SSO/GG/MBS composite films (Fig. 3A,c-e), there was no peak shifting, appearance of a new peak, or disappearance of a peak related to GG/MBS film matrix, with the exception of the peaks from the SSO. Therefore, it can be assumed that the incorporation of SSO did not affect the structure of the GG/MBS film.
XRD. An XRD analysis was performed to investigate the effect of SSO on the crystalline structure of the SSO/ GG/MBS composite films and the compatibility among the components of the films. Figure 3B presents the XRD patterns of the original materials, MBS and GG, in granule form; of the GG/MBS film; and of the SSO/GG/MBS composite films. The pattern of GG granules (Fig. 3B,a) showed three distinct peaks at 2θ = 14.3°, 17.1°, and 20.0°. In contrast, MBS granules (Fig. 3B,b) 32 . The diffraction patterns of the SSO/GG/MBS films were similar to that of the GG/MBS film without SSO. The diffractograms of all SSO/GG/MBS composite films revealed a partially crystalline nature and indicated somewhat weak diffraction peaks at approximately 2θ = 16° and 20°, which were derived from MBS and GG, respectively. This result suggests the existence of intermolecular interactions between the two polymers, i.e., a good compatibility between MBS and GG. The weak peaks observed in the diffraction pattern of the GG/MBS film (Fig. 3B,c) compared with those of the MBS and GG granules (Fig. 3B,a,b, respectively) indicated that the crystal structures www.nature.com/scientificreports/ of MBS and GG were destroyed during the film preparation. It suggested the good compatibility of the MBS and GG in the film matrix. In addition, the decrease in the crystallinity of the films was also caused by the plasticizer effect of glycerol. The glycerol incorporated in the matrix of the films was formed the intermolecular hydrogen bondings between MBS and GG. Therefore, the crystallinity of the GG/MBS film was decreased compared to the MBS and GG granules, and caused the increase in the chain mobility of MBS and GG 33,34 . Conversely, the peak intensity in the SSO/GG/MBS composite films (Fig. 3B,d-f) was decreased as SSO content increased, which suggests that the addition of SSO in the film matrix led to the formation of a less crystalline structure, thus causing a decrease in the mechanical strength of SSO/GG/MBS composite films. Similarly, Valenzuela et al. 35 also reported that the incorporation of SSO into a quinoa protein/chitosan film matrix induced a decrease in crystallinity. The reduction in the crystallinity of the SSO/GG/MBS composite films could be attributed to intermolecular interactions between the two polymers and SSO. Therefore, the SSO also increased the chain mobility of the MBS and GG, like glycerol. In other words, not only glycerol but also SSO was acting as a plasticizer in the film matrix. Meanwhile, the increase in the chain mobility in the GG/MBS and SSO/GG/MBS composite films was also affected to the OTR of the films. This issue is discussed in later subsection "OTR".
Morphological properties. An SEM analysis was carried out to study the formation and distribution of the oil droplet in the film matrix containing SSO. Figure 4 presents the SEM images corresponding to the surface and cross-section of the films. The structure of the GG/MBS film (Fig. 4A,B) without the addition of www.nature.com/scientificreports/ SSO was compact, homogeneous, continuous, and without pores. Therefore, the GG/MBS film had superior TS and EB values. In contrast, the SSO/GG/MBS composite films exhibited a rough surface and heterogeneous film structure caused by the addition of SSO. The roughness and heterogeneity of the film increased with the increasing concentration of SSO. As shown in SEM images of 0.5% SSO/GG/MBS (Fig. 4C,D) and 1% SSO/GG/ MBS (Fig. 4E,F) films, the droplet size was relatively small until the addition of 1% SSO to the GG/MBS films.
These results indicate that the SSO was well dispersed in the film matrix. However, the 2% SSO/GG/MBS film www.nature.com/scientificreports/ (Fig. 4G,H) had larger and fewer lipid globules, which trapped the SSO at both the film surface and interior. This was because of the poor dispersion of SSO droplets in the film matrix at a concentration of 2%, from the low stability of the filmogenic emulsion 36 . Therefore, the aggregation of SSO was accelerated in the film matrix during the drying process. Such an increase in film heterogeneity and decrease in miscibility caused by SSO addition were related to the degradation of the mechanical properties of the films.

otR.
The OTR values of the films are listed in Table 3. The incorporation of SSO into films caused a significant increase (P ≤ 0.05) in OTR because oxygen has a hydrophobic nature and combines well with oil. The SSO in the matrix of the SSO/GG/MBS composite films improved the oxygen dissolution, which accelerates the transfer of oxygen molecules 37 . In addition, the plasticizing effect of SSO also increased the OTR values in the SSO/GG/MBS composite films. The plasticizers reduce the resistance properties of the films to gas transmission by increasing the molecular mobility of the GG and MBS 38 . Therefore, SSO/GG/MBS composite films had significantly higher (P ≤ 0.05) OTR values compared with the GG/MBS film without SSO addition. However, there was no significant difference (P > 0.05) in OTR values between 1 and 2% SSO/GG/MBS films, despite the difference in the amount of SSO added. This result might be attributed to the effect of sweating-out of glycerol in the SSO/GG/MBS composite film ( Fig. 2A). The sweating-out phenomenon of glycerol was also discussed in the previous subsection "Optical properties". As glycerol is a hydrophilic substance, it was present on the surface of 2% SSO/GG/MBS films, which disturbed the oxygen dissolution and penetration into the film. Accordingly, despite its higher SSO content, the 2% SSO/GG/MBS film did not exhibit a significantly higher (P > 0.05) OTR value compared with the 1% SSO/GG/MBS film.
Water-resistance properties. Moisture content. The moisture content of SSO/GG/MBS composite films decreased significantly (P ≤ 0.05) with the increase in SSO content (Fig. 5A). This implies that the addition of SSO to the film matrix reduced the hygroscopicity of the films, because the hydrophobic SSO reduced the water-retention capacity of the films 39 . More specifically, fewer sites were available to bind water in the film matrix because of the increased number of hydrophobic chains 35 . In addition, the relatively decreased level of hydrophilic substances, such as MBS, GG, and glycerol, in the film matrix because of the addition of SSO may also have contributed to this tendency. Meanwhile, the moisture content of the oblate film was not significantly different (P ≤ 0.05) with that of the 2% SSO/GG/MBS films. This result was caused by the absence of glycerol in the oblate film. Glycerol is a hygroscopic plasticizer. Therefore, glycerol gives hygroscopic properties to films 40 . However, the oblate film did not include glycerol and any other hygroscopic substances, and its moisture content was relatively low.
Water solubility. The water solubility of edible films suggests their integrity in an aqueous condition 41 . The incorporation of SSO into the GG/MBS film led to a significant decrease (P ≤ 0.05) in water solubility (Fig. 5B). The addition of SSO to the film matrix at a concentration of 0.5, 1, and 2% (w/w) led to a reduction of 18.12, 27.99, and 34.80% in water solubility, respectively. These results can be attributed to the intermolecular interactions between the components of SSO and the hydroxyl groups of MBS and GG, which would reduce the possibility of interaction between hydroxyl groups and water molecules 42 . Consequently, the addition of SSO led to the enhancement of the water-resistance property of SSO/GG/MBS composite films. However, it was impossible to measure the water solubility of the oblate film because this was disintegrated in the DW after 24 h. This fact that the oblate film was very susceptible to direct contact with moisture against its low moisture content means the oblate film had relatively high water vapor barrier properties, but it had relatively low liquid water barrier properties.
WVP. The various edible films that are prepared using polysaccharides, proteins, and lipids have relatively low water-resistance properties 43 . This attribute is a drawback in the food industry as it accelerates the collapse of edible films when foods come into contact with moisture. Therefore, many researchers have focused on the improvement of the water-resistance properties of edible films 8,23,44 . The WVP is an important criterion among the various water-resistance properties of the films, as it indicates the capability of films to manage the highly humid environment at the surface of food and its surroundings. The WVP of the films depends on many various factors such as hydrophilicity or hydrophobicity of polymer materials, mobility of polymer chains, presence of cavities or cracks, structural integrity, and crystalline/amorphous ratio, type and level of plasticizer, thickness, ambient conditions (temperature and RH), and so on 45 . Changes of WVP values in the oblate, GG/MBS,   www.nature.com/scientificreports/ Meanwhile, the GG/MBS and SSO/GG/MBS composite films showed a tendency of the WVP to decrease. However, after 5 or 9 days of storage, the decrease tendency was disappeared, and WVP values in the films began to increase. This could be result of the presence of optimal (or balanced) crystalline/amorphous ratio in each film. It is reported that the barrier properties of the film were maximized when the film matrix forms the optimal crystalline/amorphous ratio. However, the crystalline/amorphous ratio in the starch-based film is constantly increased during the storage period, because of the amorphous-to-crystalline phase transition. Therefore, the WVP was decreased just prior to the crystalline/amorphous ratio in the film matrix was reached at the optimal state, and the lowest WVP values were achieved at the optimal crystalline/amorphous ratio. Since then, the crystalline/amorphous ratio gets out of the optimal state, and the WVP values in the films gradually increased. In other words, the time point when the GG/MBS and SSO/GG/MBS films showed the lowest WVP values was not immediately after fabrication but after 5-9 days of aging (or conditioning). Other researchers, Hernández-Muñoz et al. 51 and Mali et al. 52 also reported the similar tendency about the change of WVP in starch-based films during the storage period. On the other hand, the change of the WVP values in the oblate film during the storage time did not indicate the tendency to increase after decrease. This was considered because the composition of the oblate film was simpler than that of the GG/MBS and SSO/GG/MBS composite films.
WVP values in the GG/MBS and 0.5% SSO/GG/MBS films had no significant differences (P > 0.05) throughout the storage time. In addition, there were no significant differences (P > 0.05) between 1 and 2% SSO/GG/ MBS films, except for day 9. These results suggested that the addition of 1% (w/w) SSO in the GG/MBS film was most ideal for the water-resistance properties of the film.
Wettability of the film surface. The measurement of the water contact angle is a method that is used to determine the hydrophobicity or hydrophilicity of material surfaces. A high water contact angle implies greater hydrophobicity of the surface, and vice versa. Figure 5C shows the water contact angle of the oblate, GG/MBS, and SSO/ GG/MBS composite films. The oblate film had the lowest water contact value among the all film samples. Meanwhile, in the GG/MBS and SSO/GG/MBS composite films, the water contact angle of the film surfaces increased significantly (P ≤ 0.05) until the addition of 1% SSO between GG/MBS film and SSO/GG/MBS composite films but was significantly decreased (P ≤ 0.05) to the lowest value in the 2% SSO/GG/MBS film. This decrease might have been caused by the migration of the glycerol from the film inside to its surface (sweating-out) in the 2% SSO/GG/MBS films 53 (Fig. 2A). The SSO molecules decreased the intermolecular MBS-GG interactions considerably in the 2% SSO/GG/MBS film matrix. Therefore, a portion of the glycerol exuded into the film surface, which transitioned into a super-hydrophilic state because glycerol is a hydrophilic substance. For this reason, the water contact angle value was lowest in 2% SSO/GG/MBS films compared with that in all other film samples.

conclusions
This study demonstrated that the addition of SSO to the MBS-based film matrix effectively improved the overall water-resistance properties of the film. Notably, the addition of 1% (w/w) of SSO to MBS-based films reduced the water solubility and the WVP of the film at initial day (day 0) by both about 30%, and increased the water contact angle by about 10% compared with the GG/MBS film (without SSO addition). In addition, the 1% SSO/GG/MBS film had no severe side effect of SSO addition, sweating-out of glycerol. Therefore, the 1% SSO/GG/MBS film was chosen as the optimal SSO/GG/MBS composite film as it exhibited excellent overall water-resistance properties. Consequently, the results of our study suggest that the 1% SSO/GG/MBS film reported here has potential as a www.nature.com/scientificreports/ new edible film for the food-packaging industry. Nevertheless, further studies are required to assess the effect of this film in the real food system.

Data availability
The data sets generated during the current study are available from the corresponding author on reasonable request. www.nature.com/scientificreports/ Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article's Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article's Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creat iveco mmons .org/licen ses/by/4.0/.